received: 13 May 2016 accepted: 23 June 2016 Published: 25 July 2016
Controllable Phase Transformation and Mid-infrared Emission from Er3+-Doped Hexagonal-/CubicNaYF4 Nanocrystals Dandan Yang1, Dongdan Chen1, Huilin He1, Qiwen Pan1, Quanlan Xiao2, Jianrong Qiu1 & Guoping Dong1 The morphology of hexagonal phase NaYF4:Er3+ nanorods synthesized by hydrothermal method changed greatly after a continuing calcination, along with a phase transformation to cubic phase. Photoluminescence (PL) spectra indicated that mid-infrared (MIR) emission was obtained in both hexagonal and cubic phase NaYF4:Er3+ nanocrystals for the first time. And the MIR emission of NaYF4:Er3+ nanocrystals enhanced remarkably at higher calcination temperature. To prevent uncontrollable morphology from phase transformation, the cubic phase NaYF4:Er3+ nanospheres with an average size of ~100 nm were prepared via a co-precipitation method directly. In contrast, the results showed better morphology and size of cubic phase NaYF4:Er3+ nanocrystals have realized when calcined at different temperatures. And PL spectra demonstrated a more intense MIR emission in the cubic phase NaYF4:Er3+ nanocrystals with an increasing temperature. Besides, the MIR emission peak of Er3+ ions had an obvious splitting in cubic phase NaYF4. Therefore, cubic phase NaYF4:Er3+ nanospheres with more excellent MIR luminescent properties seems to provide a new material for nanocrystal-glass composites, which is expected to open a broad new field for the realization of MIR lasers gain medium. Mid-infrared (MIR) fiber lasers operating at ~3 μm are in great demand for a variety of applications including medical surgery, hazardous chemical detection, remote sensing, eye safe laser radar and atmosphere pollution monitoring1–5. This mainly relies on the two unique features of this wavelength range: (1) well-known atmospheric transparency windows are located in this wavelength range; (2) various molecules have strong rovibronic absorption lines in this ‘molecular fingerprint’ region of the electromagnetic spectrum1. So far, glass-based materials (conventional glass and glass ceramics materials) may be the most important material used for optical fiber production6–8. However, MIR emission at ~3 μm is the closely spaced energy levels transition, which is liable to be quenched by multiphonon non-radiative decay, hence, it seems difficult to obtain intense MIR emission in most glass-based materials. In comparison with glass-based materials, nanocrystal (NC) materials are thought to be more suitable as MIR laser host because of their many advantages with smaller particle size, higher chemical stability, more nature synthesis method, lower thermal lens effect and higher doping concentration of trivalent rare-earth (RE) ions9–13. Thus, in our previous work11, a novel co-melting technology has been proposed to introduce RE ions doped NC into glass matrixes to form NC-doped glass composite (NGC). The NGC can provide a stable crystalline field for active ion to realize higher MIR luminescent efficiency, and have potential for fiber-drawing, which will open a brand new field for the realization of MIR fiber lasers. NGC and co-melting technology present a new approach to research the MIR composite optical fiber preforms and fiber forming. However, the preparation of NGC brings forward rigorous demands to the MIR emission NCs, such as high MIR luminescent intensity, controllable morphology and better thermal stability etc. So it is extremely important to search suitable MIR emission NCs for NGC preparation. As an ideal host, fluorides 1
State Key Laboratory of Luminescent Materials and Devices and Institute of Optical Communication Materials, School of Materials Science and Engineering, South China University of Technology, Guangzhou 510640, China. 2SZU-NUS Collaborative Innovation Center for Optoelectronic Science & Technology, Key Laboratory of Optoelectronic Devices and Systems of Ministry of Education and Guangdong Province, College of Optoelectronic Engineering, Shenzhen University, Shenzhen 518060, China. Correspondence and requests for materials should be addressed to G.D. (email: [email protected]
) Scientific Reports | 6:29871 | DOI: 10.1038/srep29871
Figure 1. (a,b) SEM images of the as-prepared β-NaYF4 and β-NaYF4:5%Er3+ nanocrystals. (c) HRTEM image and (d) EDS spectrum of as-prepared β-NaYF4:5%Er3+ nanocrystals. (e) The MIR emission spectra of asprepared β-NaYF4 and β-NaYF4:5%Er3+ nanocrystals. The inset in (b) is corresponding SAED pattern.
with low phonon frequency and intense crystalline field, have been widely studied14–16. Among these RE fluorides, NaYF4 with low vibration energy (